Transcript of "Semiconductor Flash Memory Scaling"
Semiconductor Flash Memory Scaling
B.S. (University of Science and Technology of China) 1996
M.S. (Johns Hopkins University) 1997
A dissertation submitted in partial satisfaction of the
requirements for the degree of
Doctor of Philosophy
Engineering-Electrical Engineering and Computer Sciences
UVIVERSITY OF CALIFORNIA, BERKELEY
Committee in charge:
Professor Tsu-Jae King, Chair
Professor Vivek Subramanian
Professor Timothy Sands
The dissertation of Min She is approved:
University of California, Berkeley
Semiconductor Flash Memory Scaling
Semiconductor Flash Memory Scaling
Doctor of Philosophy in Engineering -
Electrical Engineering and Computer Sciences
University of California, Berkeley
Professor Tsu-Jae King, Chair
Semiconductor flash memory is an indispensable component of modern electronic
systems. The minimum feature size of an individual CMOSFET has shrunk to 15nm with
an equivalent gate oxide thickness (EOT) of 0.8nm in 2001. However, semiconductor
flash memory scaling is far behind CMOS logic device scaling. For example, the EOT of
the gate stack in semiconductor flash memory is still more than 10nm. Moreover,
semiconductor flash memory still requires operation voltage of more than 10V, while the
operation voltage of CMOS logic has been scaled to 1V or even less.
This dissertation addresses the issue of gate stack scaling and voltage scaling for
future generations of semiconductor flash memory, and proposes solutions based on new
memory structure and new materials that are compatible with the current CMOS process
flow. Chapter 1 discusses the key challenges in scaling flash memories. In chapter 2, a
theoretical model that accounts for both the Coulomb blockade effect and the quantum
confinement effect is proposed to model semiconductor nanocrystal memory. The
program/erase speed and retention time in terms of nanocrystal size, tunnel oxide
thickness, and different tunnel material other than silicon oxide has been investigated.
Semiconductor na nocrystal memory is shown to have the potential to replace the
conventional floating gate flash memory. Chapter 3 demonstrates that high quality silicon
nitride can be used as the tunnel dielectric to enhance the programming speed, since it
offers a low injection barrier as compared to silicon oxide tunnel dielectric. Retention
time is also enhanced due to the fact that thick tunnel nitride can be used for the same
EOT. In Chapter 4, Hafnium oxide was investigated to replace silicon nitride as the
charge trap/storage layer in SONOS (silicon-oxide- nitride-oxide-silicon) type trap-based
memory. Since the conduction band offset between Hafnium oxide and tunnel oxide is
larger than that between silicon nitride and tunnel oxide, the tunnel barrier from the
charge trap layer is reduced/eliminated during programming; fast programming speed
was achieved with Hafnium oxide trap layer experimentally. The large conduction band
offset can also improve the retention time. New device structures are also indispensable
in making flash memory more scalable. In Chapter 5, a FinFET SONOS flash memory
device has been demonstrated. Its channel length is scalable to 40nm. The experimental
results showed that the FinFET SONOS memory exhibited good program/erase speed,
high endurance and good reading disturbance. It is a suitable embedded memory for the
future FinFET circuit. FinFET memory can achieve a much smaller cell size than that
predicted by ITRS roadmap.
The dissertation abstract of Min She is approved:
Professor Tsu-Jae King Date
Table of Contents
1.1 Semiconductor memory comparison……………………………………….1
1.2 Semiconductor flash memory scaling……………………………………...5
Chapter 2 Modeling of semiconductor nanocrystal memory…………………………14
2.2 Device modeling………………………………………………………….16
2.2.1 Write/Erase modeling………………………………………………16
2.2.2 Retention time modeling………………………………………….20
2.3 Results and discussion…………………………………………………….23
2.3.1 Impact of nanocrystal size and tunnel oxide thickness on device
2.3.2 Low barrier tunnel material………………………………………26
2.3.3 Semicondcutor nanocrystal memory as DRAM………………….30
Chapter 3 Low barrier tunnel dielectrics for flash memory……………………………36
3.2 JVD nitride as a tunnel dielectric in floating gate flash memory………...36
3.2.2 Hot carrier injection efficiency………………………………….38
3.2.3 Retention and erase………………………………………………39
3.2.4 Device fabrication………………………………………………..42
3.2.5 Device characteristics……………………………………………44
3.3 Improved SONOS flash memory with thermal silicon nitride tunnel
3.3.2 Device principle……………………………………………………50
3.3.3 Device fabrication……………………………………………….…52
3.3.4 Results and discussion……………………………………………..53
Chapter 4 High-K material as charge trap/storage layer……………………………...59
4.2 Advantages of using high-k materials……………………………………61
4.3 Theoretical device modeling………………………………………….….64
4.4 HfO 2 as charge trap layer in SONOS flash memory………………….….69
4.5 TiO 2 as charge trap layer…………………………………………………75
4.6 Conclusions and discussion……………………………………………78
Chapter 5 FINFET SONOS flash memory…………………………………………..82
5.1 Introduction …………………………………………………………….82
5.2 Experiment…………………………………………………………… 86
5.3 Device characteristics…………………………………………………...90
5.4 A compact FinF ET flash memory array………………………………...99
5.7 Appendix: Process flow for FinFET SONOS flash……………………112
Chapter 6 Conclusion………………………………………………………………114
6.2 Recommendations for future work …………………………………...118
6.3 Reference…………………………………………………………….. 121
First I would like to thank my research advisor, professor Tsu-Jae King. Professor
King gave me tremendous support and invaluable advice for me to finish the graduate
study. I have benefited a lot from her continuous encouragement. I am also very
impressed by her diligence and enthusiasm for the scientific pursuit. I feel very fortunate
for the opportunity to have her as my research advisor.
I am also grateful to professor Chenming Hu, for his technical guidance throughout
my graduate research. He has been supportive of my work as well and I also enjoyed
taking his excellent courses.
I would also like to thank Professor Vivek Subramanian to serve on my qualifying
examination committer chair and my thesis committee member. I am very grateful to
both Professor Timothy Sands of the Materials Sciences department and Professor
Nathan Cheung of the Electrical Engineering department for serving on my qualifying
examination committee. I have benefited from the questions they asked during the exam
and from the interesting courses they have offered at UC Berkeley.
I am very thankful to Hideki Takeuchi, whom I admire very much. He helped me
generously in the micro- fabrication laboratory (microlab). I also had a wonderful time
with him during the cooperation on several projects. His broad knowledge and diligence
impressed me very much. I would like to thank Katalin Voros, Sia Parsa and other
microlab staffs for their technical support. I am thankful to the graduate office of the
EECS department, especially Ruth Gjerde for the efficient assistance.
I would like to acknowledge Patrick Xuan, for the collaborations on FinFET
SONOS memory. I am very grateful to Qiang Lu, Kevin Yang, Yee-Chia Yeo, Charles
Kuo, Ron Lin for the instructive technical discussions. I am indebted to the former
students or members of the Device Group, Weidong Liu, Wen-Chin Lee, Yu Cao, Kanyu
Cao, Yang-Kyu Choi, Xiaodong Jin, Jakub Kedzierski, Qing Ji, Stephen Tang, Nick
Lindert, Pushkar Ranade, Igor Polishchuk, Leland Chang, Pin Su, Xuejue Huang, for
helping me get through the initial learning stage as a new device group student.
I am also thankful to the current members of the Device Group, Alvaro Padilla, Yu-
Chih Tseng, Kyoungsub Shin, Dae-Won Ha, Hui Wan, Gang Liu, Shiying Xiong,
Donovan Lee, Joanna Lai, Hiu Yung Wong, Vid ya Varadarajan, Chung-Hsun Lin, Blake
Lin, Marie-Ange Eyoum, Katherine Buchheit, Sriram Balasubramanian, Mohan Vamsi
Dunga, Hei Kam, Dr. Jin He, Dr. Jane Xuemei Xi, Dr. Jun Lin, for their friendship and
I would like to thank Professor Yi Shi at Nanjing University, China, Professor Shinji
Nozaki at University of Electro-Communications, Japan and Professor Tso-Ping Ma at
Yale University for the discussion, help and collaboration. Their supports made my
research life enjoyable.
I would like to thank my family for their love, support and encouragement,
especially to my grandmother for the wonderful childhood I spent with her.
1.1 Semiconductor memory comparison
Semiconductor memory is an indispensable component of modern electronic
systems. It is used in personal computers, cellular phones, digital cameras, smart- media,
networks, automotive systems, global positioning systems. Table 1.1 lists the
characteristics of different types of semiconductor memory that either have been
commercialized or are being developed in the industry.
Static Random Access Memory (SRAM) is used as a cache memory in personal
computers since it offers the fastest write/read (8ns) speed among all memories.
However, a single SRAM cell consists of 6 transistors (6T), so SRAM chip density is
very low, although 4T SRAM cells have been demonstrated . SRAM memory can
retain the stored information as long as the power is on, drawing very little current.
However, the information will be lost when the power is turned off, so SRAM is not a
A Dynamic Random Access Memory (DRAM) cell consists of one transistor and one
capacitor (1T1C). It is superior to SRAM in many aspects except that the write speed is
slower in the DRAM (50ns) than in the SRAM. However, its cell size is much smaller
than that of SRAM and thus it is a low cost commodity memory device. Compared to
flash memory, DRAM has much faster program/read speed with very low operating
voltage, while flash memory needs 1us to 1ms programming time and high programming
voltage. Unfortunately, DRAM is a volatile memory. The data retention time is about
100ms in DRAM while it is 10 years in flash memory: a DRAM cell needs refreshing
frequently to maintain its data, so its power consumption is significant. Furthermore, the
size of a DRAM cell is larger than that of a flash memory cell. Scaling the DRAM cell
size down is difficult due to the large capacitor required to store data.
In the past decade, memory chips with low power consumption and low cost have
attracted more and more attention due to the booming market of portable electronic
devices such as cellular phones and digital cameras. These applications require the
memory to have ten years data retention time, so that the nonvolatile memory device has
become indispensable. There are mainly four types of nonvolatile memory technology:
flash memory, Ferro-electric Random Access Memory (FeRAM* ), Magnetic Random
Access Memory (MRAM) and phase change memory. Flash memory is presently the
most suitable choice for nonvolatile applications for the following reasons:
1) Flash memory can achieve the highest chip density. A flash memory cell consists
of only one transistor . A FeRAM memory cell generally consists of one transistor
and one capacitor , while a MRAM cell needs a transistor and a magnetic tunnel
junction . Phase change memory was expected to be a promising nonvolatile
memory ; however, its memory cell consists of one resistor and a bipolar junction
transistor. Until now, only a 4MB phase change memory chip has been demonstrated.
It will take more effort to demonstrate whether the phase change memory is really a
FeRAM is not a perfect nonvolatile memory since its reading mode is destructive. A
programming verification is required to restore the data after reading.
Memory type DRAM SRAM Flash- Flash- FRAM MRAM Phase
NOR NAND change
Cell size 6~12 90~150 8~10 4 18 10~20 5~8
factor (F2 )
Largest array 256 2Gb 64 1 4
Volatile/Non- Volatile Volatile NV NV NV NV NV
Endurance ∞ /∞ ∞ /∞ 106 / ∞ 106 / ∞ 1012 / 1012 1014 / ∞ 1012 / ∞
Read Destructive Partially- Non- Non- Destructiv Non- Non-
destructive destructi destructi e destructive destructive
Read/Progra ~1 ~1 2/10 2/18 1.5/1.5 3.3/3.3 0.4/1
m voltage (V)
Program/Eras 50/50/8 8/8/8 1us/1- 1ms/1- 80/80/80 30/30/30 50/50/50
e/Read speed, 100ms 100ms/60
ns (block)/6 ns
Direct over- Yes Yes No No Yes Yes Yes
Bit/byte Yes Yes Yes Block Yes Yes Yes
Read 100- 100- Delta Delta 100- 20-40% R 10X-100XR
dynamic 200mV 200mV current current 200mV
Programming Medium Medium High Low Medium Medium Low
Transistors Low High High High Low High High
performanc performanc voltage voltage performan performanc performance
e e ce e
CMOS logic Bad Good Ok, but Ok, but Ok, but Hi Good
compatibility Hi V Hi V V needed
New Yes No No No Yes Yes Yes
Scalability Capacitor 6T (4T Tunnel Tunnel Polarizable Current Lithography
limit possible) oxide/HV oxide/HV capacitor density
Multi-bit No No Yes Yes No No No
3D potential No No Possible Possible ? ? No
SER Yes Yes No No Yes No No
Relative cost Low High Medium Medium High ? Low
Extra mask 6-8 2 4 3-4
In production Yes yes Yes Yes Yes 2004 N/A
Table 1.1: Performance Comparison between volatile memory (DRAM and SRAM)
and nonvolatile memory (Flash, FRAM, MRAM and phase change memory) devices.
Among the nonvolatile memories, flash memory is the only memory compatible with
the current CMOS process flow. Overall, the flash memory exhibits the best
performance except for the disadvantages of high programming voltage and slow
2) Flash memory possesses the multi-bit per cell storage property . Four distinct
threshold voltage (VT ) states can be achieved in a flash memory cell by controlling the
amount of charge stored in its floating gate. Two-bits/cell (with four VT states) flash
memory cells have already been commercialized. A four-bits/cell flash memory device
is feasible and is under development now . Multi-bit storage increases memory
density and thus reduces the cost per bit significantly. Furthermore, Matrix
Semiconductor Inc. demonstrated multi- layer (sometimes called “three-dimensional
integration”) SONOS flash memory recently . This novel idea offers another
possibility to achieve even higher density and lower cost technologies based on flash
A 2GB NAND-type flash memory chip has been demonstrated in . A plot of the
NOR-type flash memory cell size versus technology generation is shown in Fig1.1
(with FeRAM as a comparison). At the 130nm generation, a FeRAM memory cell is
Cell size (um )
0.01 year of 2004
160 140 120 100 80 60 40 20
Figure 1.1: Cell size comparison between flash memory and FeRAM. Flash memory
has the smallest cell size among all of the nonvolatile memories. The data is from
the 2002 International Technology Roadmap for Semiconductors.
as 26 times larger than its flash memo ry counterpart.
3) Flash memory fabrication process is compatible with the current CMOS process
and is a suitable solution for embedded memory applications. A flash memory cell is
simply a MOSFET cell, except that a poly-silicon floating gate  (or Silicon Nitride
charge trap layer ) is sandwiched between a tunnel oxide and an inter-poly oxide to
form a charge storage layer. All other nonvolatile memories require integration of new
materials that are not as compatible with a conventional CMOS process. It is easier
and more reliable to integrate flash memory than other nonvolatile memories with
logic and analog devices in order to achieve better chip performance for wireless
communication and wireless computation .
Since flash memory possesses these three key advantages, it has become the
mainstream nonvolatile memory device nowadays.
However, flash memory exhibits some evident disadvantages as shown in Table 1.1:
the device has a slow program/erase speed and requires a high voltages to program/erase
its data. Additionally, its endurance also needs to be improved, although 105
program/erase cycles is enough for most applications. This thesis will investigate several
ways to improve the program/erase speed and reduce the operation voltage.
1.2 Semiconductor flash memory scaling
The minimum feature size of an individual CMOSFET has shrunk to 15nm with an
equivalent gate oxide thickness (EOT) of 0.8nm in 2001, . However, semiconductor flash
memory scaling is far behind CMOS logic device scaling. For example, the EOT of the gate stack
in semiconductor flash memory is still more than 10nm. Moreover, semiconductor flash memory
still requires operation voltages of more than 10V, while the operation voltage of CMOS logic has
been scaled to about 1V or even less.
It is important to scale the EOT of the gate stack to achieve a small memory cell size,
and also prolong battery life. A floating gate flash memory structure is shown in Fig 1.2.
The gate stack consists of an 8nm thermal oxide as the tunnel layer, a 150nm poly-silicon
floating gate and a 13nm (EOT) inter-poly oxide layer . The EOT of the whole gate
stack is 21nm. A typical drain bias is 2V in the reading mode and 4.5V in the
programming mode. This memory cell suffers from serious short channel effects when
the channel length is scaled to sub 100nm, since the EOT of the gate stack is very thick
and the drain bias is relatively large. Both the drain- induced barrier lowering (DIBL)
effect and the sub-surface punch-through effect induce significant leakage current during
reading and programming. As shown in Fig 1.3, the leakage current contributed by the
unselected cells along the same bit line may be so significant that the sensing circuit
thinks the selected cell is at a low threshold voltage (VT ) state (with high reading current)
although the selected cell actually is at a high VT state (with low reading current). During
programming, the leakage current may be very significant so that it causes significant
Tunnel oxide Floating Gate
Figure 1.2: Schematic cross-section of a floating gate memory device. It is
essentially a MOSFET, except that a floating gate is sandwiched between a tunnel
oxide and an inter-poly oxide. The tunnel oxide must be thicker than 8nm to
maintain 10 years retention time at 85o C.
The high voltages required for operation inhibit memory chip density improvement.
A flash memory chip consists of two parts: the core memory cells, and the peripheral
micro-controller circuit. Many high voltage transistors are used in the peripheral circuit to
produce the high voltage required to program/erase the core memory cells. These high
voltage transistors consume a lot of area. In the 0.18um technology generation, the
BL j-1 BL j BL j+1
Selected cell Unselected cell
Figure 1.3: Word line (WL) i and bit line (BL) j are biased in reading mode to read the
selected memory cell (i, j). The current leakage from the unselected cells along the same
bit line j may contribute significant current to cause a wrong reading of cell (i, j).
peripheral circuit occupies an area on the chip that is comparable to the area required for
the core memory. The peripheral circuit scales more slowly than the core memory, since
the operation voltages have not been scaled down over the past several technology
generations. The peripheral circuit also consumes a lot of power to generate the high
WL i-1 WL i WL i+1
Selected cell Unselected cell
Figure 1.4: The spacing (100nm shown in the figure) between the word lines has to
be scaled down further to increase the core memory density. During programming of
the selected cell (WL i-1 biased at 10V), word line i is also turned on due to
capacitive coupling, so the unselected cell is also programmed. This cross coupling
is more severe as the spacing between word lines is decreased, thus limiting the
scalability of the word line spacing.
Furthermore, the high voltage operation has a direct impact on the core memory
array scaling. Fig 1.4 shows the NROM memory array layout . The poly-silicon
word lines (WL) should be patterned as close as possible to each other to reduce the
memory array size. Unfortunately, the poly-silicon word lines will suffer serious
capacitive coupling when the spacing between them is reduced. Since the poly-silicon
word line is usually very long (several tens of microns), the cross coupling is very strong.
If either word line i-1 or word line i+1 is turned on (or both word lines are on at the same
time), word line i will be turned on too, due to the cross coupling effect. Then, the
unselected cell will be erroneously programmed.
The scaling of the gate stack and operation voltages are often related to each other.
A tunnel oxide thickness of more than 8nm is currently used in the commercial flash
memory chip to meet the ten years data retention time requirement. If the tunnel oxide
were to be scaled below 2nm, the operation voltage could be reduced from more than
10V to below 4V . Unfortunately, the retention time would also be reduced, from 10
years to several seconds.
Year of production 2004 2007 2010 2013 2016
Technology node (nm) 90 65 50 35 25
Flash NOR Lg(um) 0.2-0.22 0.19-0.21 0.17-0.19 0.14-0.16 0.12-0.14
Flash NOR highest
W/E voltage (V) 7-9 7-9 7-9 7-9 7-9
Flash NAND highest
Voltage (V) 17-19 15-17 15-17 15-17 15-17
NOR tunnel oxide(nm) 8.5-9.5 8-9 8-9 8 8
NAND tunnel oxide(nm) 7-8 6-7 6-7 6-7 6-7
Solution exist Solution known Solution NOT known
Table 1.2: Tunnel oxide and operation voltage scaling predicted by the 2002 International
Technology Roadmap for Semiconductors.
Table 1.2 shows the 2002 International Technology Roadmap for Semiconductor
flash memory . The channel length of the NOR type flash memory will still be longer
than 100nm by the year 2016. Short channel effects prevent the channel length from
being aggressively scaled. The operation voltage and the tunnel oxide will not scale at all
in the coming five technology generations.
This dissertation addresses the aforementioned issue of gate stack scaling for
future generations of semiconductor flash memory, and proposes solutions based on new
memory structures and new materials that are compatible with the current CMOS process
flow. Chapter 2 discusses the scaling limit of semiconductor nanocrystal memory
devices. After an introduction of the general scaling requirement for tunnel oxide, a
theoretical model taking into account the quantum confinement effect and the Coulomb
blockade effect is proposed to explain the program/erase and retention characteristics of a
nanocrystal memory. The effect of nanocrystal size, tunnel oxide thickness and tunnel
material on the device performance is investigated. It is concluded that semiconductor
nanocrystal memory is a promising nonvola tile memory although a more delicate
fabrication method is required to achieve uniform nanocrystal size.
In Chapter 3, high quality Jet vapor deposited (JVD) silicon nitride is proposed as a
tunnel dielectric in floating gate flash memory. The hot electron injection barrier at the
interface between the JVD nitride and the silicon substrate is 2.12eV, which is much
lower than the 3.15eV injection barrier offered by a thermal silicon oxide tunnel
dielectric. More efficient electron injection is expected during programming with JVD
nitride tunnel dielectric. After hot carrier injection efficiency is discussed, the device
operation principle and fabrication process are shown. Then, the device performance is
presented. A comparison between JVD nitride and thermal oxide as a tunnel dielectric is
made in terms of program/erase speed, retention, programming disturbance and so on.
High quality silicon nitride can also be a tunnel dielectric in a trap-based flash
memory. In Chapter 3, thermal silicon nitride is used as a tunnel dielectric in a SONOS-
type (polysilicon-oxide-nitride-oxide-silicon) memory device. The principle of silicon
nitride as the tunnel dielectric in trap-based memory is different from the JVD nitride as
the tunnel dielectric in floating gate flash memory. The device fabrication and
characterization are presented. Although the thermal silicon nitride is thinner than
required due to fabrication limitations (so the memory is not nonvolatile), initial results
show that high quality silicon nitride can still be a promising tunnel dielectric for trap-
based nonvolatile memory applications.
Instead of scaling the tunnel oxide, new charge trap/storage materials can also be
used to improve the programming speed at low operation voltage and improve the
retention at the same time. In Chapter 4, a high electron affinity, high-K dielectric is
investigated as a charge trap layer to replace the conventional LPCVD silicon nitride trap
layer in the SONOS-type flash memory. To be integrated in flash memories, these new
charge trap materials should be thermally stable during high temperature processes, in
addition to providing deep trap energy levels and sufficient trap density. A memory
device with hafnium oxide charge trap layer shows faster programming speed than a
device with silicon nitride charge trap layer and good retention.
Chapter 5 proposes a double-gate “FinFET” SONOS flash memory for embedded
silicon-on- insulator (SOI) application. The FinFET flash memory demonstrates similar
performance as the bulk SONOS flash memory, although there is no body contact in the
FinFET device. Good sub-threshold swing is achieved with the FinFET structure, so that
the ratio of reading current between the selected cell and the unselected cell is increased.
Memory devices fabricated with (100) channel surface and (110) channel surface are
compared in terms of program/erase speed and retention. A high-density memory circuit
is proposed to achieve a very small cell size for sub 100nm technology generation.
The dissertation is concluded with a summary of the major results and possible
future research directions in Chapter 6.
 “Advanced Memory Technology and Architecture”, short course, IEDM 2001.
 Seiichi Aritome, “Advanced Flash Memory Technology and Trends for Files Storage
Application”, pp.763, IEDM 2002.
 D.J. Jung, “Highly Manufacturable 1T1C 4Mb FRAM with Novel Sensing Scheme”,
pp.279-282, IEDM 1999,
 S. Lai and T. Lowrey, “OUM- A 180nm Nonvolatile Memory Cell Element
Technology for Stand Alone and Embedded Applications”, pp.803, IEDM 2001.
 Paolo Cappelletti, “Flash Memories”, Kluwer Academic Publishers, 1999.
 Pier Luigi Rolandi et al, “A 4-bit/cell Flash Memory Suitable for Stand-Alone and
Embedded Mass Storage Applications”, pp.75, Non-Volatile Semiconductor Memory
Workshop, Monterey, CA 2000.
 A.J. Walker et al, “ 3D TFT-SONOS Memory Cell for Ultra-High Density File
Storage Applications”, 2003 Symposium on VLSI Technology.
 D.C. Kim et al, “ A 2Gb NAND Flash Memory with 0.044 um2 Cell Size using 90nm
Flash Technology”, pp.919-922, IEDM, 2002.
 Takuya Kitamura et al, “ A Low Voltage Operating Flash Memory Cell with High
Coupling Ratio Using Horned Floating Gate with Fine HSG”, pp.104-105, 1998
Symposium on VLSI Technology.
 A.Fazio, “0.13um Logic+Flash: Technology and Applications”, Non-Volatile
Semiconductor Memory Workshop, Monterey, CA 2000.
 B.Yu, “15nm Gate Length Planar CMOS Transistor”, pp.937-939, IEDM, 2001.
 B.Eitan et al, “NROM: A novel localized trapping, 2-bit nonvolatile memory cell”
pp. 543-545, Vol.21, Issue 11, IEEE Electron Device Letters, 2000.
 Y. King, “Thin Dielectric Technology and Memory Devices”, Ph.D dissertation,
Univ. of California, Berkeley, CA 1999.
“International Technology Roadmap for Semiconductors, 2002 update” at
Modeling of semiconductor nanocrystal
Aggressive scaling of semiconductor memory cells and the dramatic increase in the
memory array size demand a high density, low cost, and low power consumption cell
structure. It is hard to scale a DRAM cell with a large capacitor. Frequent refreshing in
DRAM results in large power consumptio n. Flash EEPROM does not require refreshing
and thus consumes less power and achieves much higher array density with a stacked
floating gate structure. However, Flash EEPROM is much slower to program and has poor
endurance. In order to improve the write/erase speed of a floating- gate device, the
thickness of the tunnel oxide must be reduced. The tunnel oxide must be less than 25Å in
order to achieve 100 ns write/erase time for a reasonable programming voltage (<10 V)
. Unfortunately, the retention time will be too short then. Stress- induced leakage current
(SILC) will further degrade the retention time. Currently, commercial flash memory
devices use tunnel oxide thicker than 8nm to guarantee 10 years retention time, which
results in high programming voltage and slow programming speed.
To alleviate the tunnel-oxide design trade-off for floating- gate memory devices, a
single-transistor memory-cell structure with discrete nanocrystal charge-storage sites
embedded within the gate dielectric was proposed . The possibility of exceeding the
performance limits of the conventional floating- gate device spurred many subsequent
investigations into this approach. In the conventional floating-gate flash memory, if there
is one defect chain across the tunnel oxide, all of the charges stored on the floating- gate
will leak back to either the channel or the source/drain though the defect chain. The
floating gate memory requires thick tunnel oxide to prevent charge loss through the defect
chain. The serious leakage problem during retention can be eliminated by utilizing a
semiconductor nanocrystal memory structure. Only the electrons stored on the nanocrystal
directly above the defect chain will be affected since the nanocrystals are separated from
each other within the gate oxide dielectric. Hence the tunnel oxide thickness in the
nanocrystal memory device can be reduced to allow faster programming and lower voltage
operation. Various techniques have been developed to form the nanocrystals in the gate
oxide. For example, Kim et al. employed LPCVD to fabricate Si nanocrystals with 4.5
nm average size and an areal density of 5×1011 cm-2 . King et al. fabricated Ge
nanocystals by oxidation of a Si1 -x Gex layer formed by ion implantation, and demonstrated
quasi- nonvolatile memory operation with a 0.4 V threshold-voltage shift . Although the
performance of nanocrystal memory devices with various nanocrystal sizes and
tunnel/control oxide thicknesses has been experimentally investigated, no theory is
available to guide the design of nanocrystal memory devices or to predict their
performance limits. In this Chapter, a theoretical model that accounts for both the
Coulomb blockade effect  and the quantum confinement effect is proposed to calculate
the write/erase speed in terms of germanium (Ge) nanocrystal size, tunnel oxide thickness,
and different tunnel material other than silicon dioxide, followed by a trap model to
describe the retention. The impacts of nanocrystal size and tunnel-oxide thickness are
analyzed, and the suitability of nanocrystal memory devices for nonvolatile memory and
DRAM applications is discussed.
2.2 Device modeling
2.2.1 Write/Erase modeling
The write and erase processes for an n-channel semiconductor nanocrystal memory
device are illustrated schematically in Fig. 2.1(b) and 2.1(c).
T2 D T1
Control Tunnel source Ec
gate(poly) oxide SiO2
Et “write “
oxide Si-sub Tunnel
Figure 2.1: (a) Schematic cross-section of nanocrystal memory device structure; (b)
illustration of write process: inversion- layer electron tunnels into the nanocrystal; (c)
illustration of erase process: accumulation layer hole tunnels into the nanocrystal, electron
in nanocrystal can tunnel back to the channel.
During the write process, a positive gate voltage is applied to inject channel
inversion-layer electrons into the nanocrystals. During the erase process, a reverse gate
bias is applied to cause the electrons to tunnel back into the channel and the accumulation-
layer holes to tunnel into the nanocrystal from the channel. To simplify the theoretical
analysis, the control oxide thickness T2 is fixed at 50Å, unless otherwise mentioned. This
thickness is enough to block the electron and hole tunneling between the control gate and
the nanocystal. Hence tunneling across the control oxide layer is neglected. It is assumed
that the nanocrystals are well separated (by greater than 5 nm) so that lateral tunneling
between nanocrystals can be neglected, which is essential for enhancing the retention time
compared with the conventional floating gate flash memory. The time-dependent
tunneling current density between the two-dimensional electron gas (2DEG) and the
nanocrystal during the write process can be expressed as:
J (t) = e ∑ g i ∫ P( E ) f j ( E) ρi ( E) f ( E) dE (2.1)
i, j E ≥ E cn
P(E) transmission probability across the tunnel oxide calculated with WKB
i index for the two degenerate valleys (total six valleys) of the conduction band;
j index of sub-band for each conduction band valley;
ρ i (E) density of states for each valley;
f (E ) fermi distribution;
gi the degeneracy for these two degenerate valleys;
f j (E ) impact frequency of the electrons impinging on the tunnel layer/silicon substrate
Ecn conduction band edge in the nanocrystal.
Assuming a triangular electrostatic potential at the silicon substrate, the impact
frequency can be expressed as
F j (E ) = ( m z E j / 3) −1 / 2 (2.2)
Here E si is the silicon surface electrical field, ε si is the silicon dielectric constant,
m z is the silicon electron effective mass along the (100) direction, and E j is the j-th
sub-band bottom energy. The electric field and sub-band bottom energy in terms of
applied gate voltage are calculated using a quantum simulator developed at the University
of California at Berkeley . Only electrons with energies higher than the nanocrystal
conduction band edge Ecn can tunnel into the nanocrystal. The total charge on the
nanocrystal is expressed as:
Q= ∫ J (t )Adt (2.3)
Where t w is the write pulse time and A is nanocrystal capture cross section area.
The injection current is time-dependent since the electric field across the tunnel oxide
depends on the charge in the nanocrystal. The coulomb blockade effect will be explained
first followed by the quantum confinement effect. When one electron is stored, the
nanocrystal potential energy is raised by the electrostatic charging energy e2 /2C, where C
is the nanocrystal capacitance, which depends mainly on the nanocrystal size, though it
also depends on tunnel oxide thickness and control oxide thickness. The capacitance is
self-consistently calculated using an electrodynamics method . The electron charge
will raise the nanocrystal potential energy and reduce the electric field across the tunnel
oxide, resulting in reduction of the tunneling current density during the write process. For
a nanocrystal of 3nm diameter, 2.5nm thick tunnel oxide and 5nm thick control oxide, the
electrostatic charge energy will be 95meV if there is one electron on the nanocrystal. If
there are two electrons, this charging energy can be 380meV, which is so high that the
second electron will have difficulty tunneling across the tunnel oxide layer. The Coulomb
blockade effect has both advantages and disadvantages. It is more dominant at low
programming voltages (<3V). In a flash memory array, device cells often encounter
disturbances with low gate voltage soft-programming. The Coulomb blockade effect can
effectively inhibit the electron tunneling at low gate voltage and improve the flash
memory array immunity to disturbance. On the other hand, the Coulomb blockade effect
should be reduced by employing large nanocrystals if large tunneling current and fast
programming speed are desired. The Coulomb blockade effect has a detrimental effect on
the retention time, since the electrons in the nanocrystal have large tendency to tunnel
back into the channel if the nanocrystal potential energy is high in retention mode.
The quantum confinement effect becomes significant when the nanocrystal size
shrinks to the nanometer range, which causes the conduction band in the nanocrystal to
shift to higher energy compared with bulk material . The quantum confinement energy
dependence on nanocrystal size has been studied both experimentally and theoretically
with the tight-binding model . Compared with bulk Ge, a 3nm Ge nanocrystal can
have a conduction band shift of 0.5eV, which is significant enough to affect the electrical
performance of the nanocrystal memory cell. In the energy band diagram shown in
Fig.2.1, the Coulomb blockade charging energy only raises the electrostatic potential of
the nanocrystal; the quantum confinement energy shifts the nanocrystal conduction band
edge upward so that the conduction band offset between the nanocrystal and the
surrounding oxide is reduced.
The material properties of the oxide tunnel dielectric are shown in Table 2.1. The
conduction band energy shifts for 5, 3 and 2 nm nanocrystal size are taken as 0.15, 0.5 and
1 eV respectively, which are the average values from several experimental sources
. These values are close to the published data calculated from the tight binding
model . For the erase process, the accumulation- layer holes tunneling into the
nanocrystal valence band are calculated similarly to calculating the write process. The
valence band energy shifts of the nanocrystals are 0.25, 0.49 and 0.78eV for 5, 3 and 2nm
nanocrystal size, respectively. The times required to charge each nanocrystal with one
electron and one hole are defined as the write time and erase time, respectively. The
capture area is approximated as the physical cross-section of the nanocrystal.
Tunnel layer me /m0 mh /m0 electron hole barrier Dielectric
barrier (eV) (eV) constant
Oxide 0.5 0.5 3.15 4.5 3.9
Nitride 0.5 0.41 2.12 1.9 6.9
Table 2.1: tunnel dielectric material properties.
2.2.2 Retention time modeling
During the retention mode, the electrons inside the nanocrystal can not be stored in
the conduction band for several reasons. First, the conduction band edge inside the
nanocrystal is higher than that of the substrate because of the charging effect and quantum
confinement effect, which allows electrons to tunnel back to the channel very easily. This
is not consistent with the long retention time observed in the published experimental data
. Second, the experimental retention time measurement shows large temperature
dependence even in the narrow temperature range between room temperature and 85o C
. If the electrons are stored in the nanocrystal conduction band, the retention time
should only show mild change between room temperature and 85o C, even if the
conduction barrier height dependence on temperature is taken into account . Third, the
memory phenomenon disappears if the semiconductor nanocrystal memory device is
annealed in hydrogen . This suggests that there are many deep trap states such as a Pb
center in the nanocrystal . The electrons will fall into in the deep traps after they
tunnel into the nanocrystal conduction band. The trap model proposed here can also
explain the long retention time observed and the large temperature dependence of
retention time. In this paper, the trap model will be described first. Then the trap energy
level will be extracted from experimental data . Finally the retention time in terms of
tunnel oxide thickness will be examined to study the suitability of nanocrystal memory
devices for nonvolatile memory and DRAM applications.
After an electron is injected into the nanocrystal, it will fall into the trap states through
some scattering mechanism. During erasing or retention, electrons will be thermally de-
trapped to the conduction band and will then tunnel back to the channel.
The probability of an electron escaping from the deep trap states back to the channel
is described as
E + Et
P(t ) = ∫ αP( E) f imp ( E) exp( − )ρ ( E ) dE (2.4)
E > Ecn kT
E + Et
Here, P( E) is the transmission probability across the tunnel oxide, and exp( − ) is
the de-trapping efficiency from the deep trap level into the conduction band, where E t is
the relative trap energy level below the conduction band. f imp (E) is the Weinberg impact
frequency expressed as ( E + Es ) / h that describes the escape frequency of the electron
from the conduction band. Es is the quantum confinement energy that is equal to the
conduction band energy shift mentioned earlier. The electron can impinge on the
nanocrystal/oxide interface from all directions. Only the perpendicular component of the
Weinberg impact frequency is effective in the retention time calculation, as shown in Fig
2.2. Therefore a factor α is included to take into account the geometry effect. It can be
treated as a fitting parameter for any nanocrystal shape.
fimp Figure. 2.2: Illustration of the geometry
control effect. Electron impinges on the nanocrystal
substrate surface in every direction.
During retention mode, the electric field across the tunnel oxide is very small and the
accumulation- layer hole density is negligible so that there is no significant hole tunneling
into the nanocrystal. Hence only electron tunneling back into the channel is considered
during retention mode. Then the time dependence of the charge in the nanocrystal can be
dQ ( t ) / dt = −P( t )Q ( t ) (2.5)
Q(t ) = Q(0) e − ∫ P (t ) dt (2.6)
From the above expression, the remaining charge on the nanocrystal can be calculated
in terms of time and temperature. The retention time is defined as the time when 20% of
the charge leaks at zero gate bias. In this thesis, the deep trap energy level is assumed to
be independent of the nanocrystal size. This assumption is reasonable since the trap
energy level depends mainly on the bonding distortion at the nanocystal/surrounding
dielectric interface . The bonding distortion should depend on the nanocrystal shape,
the nanocrystal material and the tunnel dielectric material, rather than nanocrystal size.
2.3 Results and discussion
The deep trap energy level and the geometry factor in Equation (2.4) are extracted
from the experimental retention data . Since the retention time depends on temperature
as shown in Equation (2.4), the deep trap energy level E t can be fitted with the
experimental retention data obtained at room temperature and 85o C, as shown in Fig.2.3.
The deep trap energy level E t and the geometry factor α are extracted to be 0.51eV and
trap model (E t=0.51eV)
10 D=3nm, T1 =15A
Retention time (sec)
20 40 60 80 100 120
Temperature ( C)
Figure 2.3: The trap energy level and the geometry effect can be determined by fitting
with experimental data.
2.3.1 Impact of Nanocrystal size and tunnel oxide thickness on device performance
Programming time (sec)
1 T1=30A Figure 2.4: The write/erase
-1 erase characteristics for various tunnel oxide
thicknesses T1 , for 3nm nanocrystal.
10 Fast programming speed can be
10 achieved at low programming voltage.
-10 -8 -6 -4 -2 0 2 4 6 8 10
Gate Voltage (V)
Fig. 2.4 shows the write/erase (W/E) characteristics as a function of gate voltage for
various tunnel-oxide thicknesses, for 3 nm-diameter Ge spherical nanocrystals. At a 20 Å
tunnel oxide thickness, the write speed can reach 100ns at programming voltage of 10 V.
For a thicker tunnel oxide of 30 Å, a write speed of 10 µs can be achieved at 10V
10 retention at 85 C
10 write at 5V
10 write at 10V
20 22 24 26 28 30
tunnel oxide thickness (A)
: Rete Figure 2.5: Programming and retention time vs. tunnel oxide thicknesses, for various
nanocrystal sizes. For 5nm nanocrys tal, 25 Å tunnel oxide can guarantee 10 years
retention time and 1 µs programming speed can be maintained at 10V.
Semiconductor nanocrystal memory can work as a flash memory exceeding the
performance of conventional floating gate memory.
Fig. 2.5 shows the retention time versus the tunnel oxide thickness for various
nanocrystal sizes. A tunnel oxide of 28 Å is thick enough to guarantee 10 years retention
time at 85o C for a 3nm nanocrystal. The impact of nanocrystal size on write/retention
performance is also shown. The characteristics for nanocrystals of 2nm, 3nm and 5nm
diameter are compared. As shown in Fig. 2.4, 5nm nanocrystals can be programmed
fastest and have better retention time at all tunnel oxide thicknesses. Larger diameters
favor electron charging due to small quantum confinement/Coulomb-charging effects, and
hence larger tunneling probability. Quantum confinement effects dominate for D smaller
than 5 nm, because the quantum confinement energy is approximately inversely
proportional to the square of nanocrystal diameter (or radius) while the Coulomb charging
energy is only inversely proportional to the diameter. For faster programming speed, large
nanocrystal size is desirable. However as mentioned before, it is desirable to reduce the
nanocrystal size for better reliability (stress induced leakage during retention). So there is
a trade-off between programming speed and reliability in selecting the nanocrystal size.
The quantum confinement energy in a 5nm nanocrystal is only 0.15eV, which is already
very small. The Coulomb charging effect cannot be reduced significantly unless very large
nanocrystals (>20nm) are utilized. Hence 5nm diameter nanocrystals would be a good
choice for practical application of nanocrystal memory devices. It is evident from Fig. 2.4
that the tunnel oxide thickness can be reduced to 25 Å to guarantee 10 years retention with
5nm nanocrystals, and a 1 µs programming speed can be maintained at 10V. The
retention/programming time ratio is at least 106 times larger than that of floating gate
flash memory in this case .
2.3.2 Low barrier tunnel material
Recently low barrier, high-K materials such as jet vapor deposited (JVD) nitride have
been demonstrated to be good tunnel dielectrics for flash memory devices . High-K
materials offer three advantages: low barrier results in larger tunneling current and hence
improves programming speed; high-K constant reduces the charging energy; deep trap
energy level can be obtained with the high-K material . The write/retention
characteristic in terms of tunnel nitride thickness is shown in Fig. 2.6.
10 D=5nm, T =50A
10 write at 5V
10 write at 10V
Retention at 85 C
10 15 20 25 30
Tunnel nitride thickness (A)
Figure Figure2.6: The retention time and write speed vs. the nitride tunnel layer
The relative trap energy level (0.51eV) is assumed to be the same as that in a thermal
oxide tunnel dielectric. Figure 6 shows that the nitride tunnel layer of 28 Å is enough to
guarantee 10 years retention time at 85o C, while achieving 18 ns write speed at a
programming voltage of 10V. Fig. 2.7 shows a comparison of the write speed obtained
with different tunnel dielectrics. For a certain specified retention time (for example, 10
years), the nitride tunnel layer memory is much faster because the electron injection
barrier of the nitride is only 2.12eV, which is much lower than the 3.15eV barrier of
oxide. In the Fowler-Nordheim (10V programming voltage) tunneling regime, the
tunneling current depends strongly on the injection barrier height. High-K tunnel
dielectrics can provide deeper trap energy level . If E t is taken to be 0.8eV, then the
nitride tunnel layer memory can be programmed much faster than the oxide tunnel layer
memory even at a programming voltage of 5V, since the nitride thickness can be reduced
further for a specified retention time.
Oxide tunnel layer, E t=0.51eV
10 Nitride tunnel layer, Et=0.51eV
-6 Nitride tunnel layer, Et=0.8eV
Write speed (sec)
10 4 5 6 7 8 9 10
10 10 10 10 10 10 10
Retention time (sec) 10 years
Figure 6 F Figure 2.7: The write speed comparison of nitride tunnel layer and oxide tunnel
layer memories. The nitride layer memory has much faster programming speed at
large gate bias. The tunnel nitride layer thickness can be reduced if the trap
energy level is 0.8eV, which result in enhanced programming speed.
To illustrate the role of the charging energy reduction obtained by using high-K
dielectrics, the programming speeds of 2nm Ge nanocrystal embedded in nitride vs. oxide
dielectric are compared, since the charging energy for 5nm nanocrystal embedded in oxide
is only about 50meV. As shown in Fig. 2.8, the oxide and nitride tunnel layer thicknesses
are chosen to guarantee 10 years retention time while the charging energies are 154.7meV
and 77.9meV, respectively. A tunnel nitride thickness of 40Å is needed to guarantee 10
years retention time because of the large quantum confinement energy of a 2nm
nanocrystal. At large programming voltage (>7V), the nitride memory programming speed
is much faster due to the lower tunneling barrier. For small programming voltage (<4V),
the nitride tunnel layer memory programming speed is slower since the nitride tunnel layer
is very thick. The disadvantage of the large physical thickne ss outweighs the benefit from
the reduction of the charging energy obtained by using a nitride tunnel layer. If the
charging energy of a nanocrystal embedded in nitride is assumed to be 154.7meV, the
programming speed of the nitride memory is at least one order of magnitude slower than
what it ideally should be. Reduction of the charging energy improves the programming
speed, but the improvement is overwhelmed by the disadvantage of the larger physical
nitride thickness required for retention.
8 D=2nm, T2=50A (EOT)
10 Ec:charging energy
Programming time (sec)
10 Figure 7: Figure 2.8: The reduction of charging
T1=30A SiO2 ,Ec=154.7meV
T1=40A Si3N4, Ec=77.9meV energy achieved by using nitride
2 T1=40A Si3N4, Ec=149.8meV tunnel dielectric helps the
10 programming speed, although it is
10 overwhelmed by the disadvantage of
-2 the thicker tunnel nitride thickness
-4 needed for retention.
2 3 4 5 6 7 8 9 10
Recently a multiple tunnel layer stack was proposed to improve the programming
speed . Although the reliability of the multi- tunnel layer is questionable, a bi- layer
tunnel dielectric consisting of thermal oxide/HfO 2 is investigated here to see if it could be
applied in the semiconductor nanocrystal memory. HfO 2 has very low electron injection
barrier of 1.5eV and high dielectric constant of 24. The electron effective mass inside
HfO 2 is taken to be 0.11m0 . The energy band diagram during write/retention is shown in
Fig. 2.9. During a write operation, the energy band of the HfO 2 is below that of the silicon
substrate so that HfO 2 won’t block electron injection into the nanocrystal. Since the
electric field during retention is very small, HfO 2 blocks electron tunneling back to the
substrate very efficiently. So both the programming speed and the retention time can be
The comparison of a bi- layer tunnel dielectric and single oxide tunnel layer is shown
in Fig. 2.10. The bi- layer offers faster programming speed for programming voltage above
4.2V. For instance, the programming speed is 200ns at 6V; that is much better than the
140 µs speed of single oxide tunnel memory. Also, the retention of the multi-tunnel layer
memory is 800 times longer than the single tunnel layer memory (not shown here).
(1) (2) (3) (4)
SiO 2 “write “
Figure 2.9: Energy band diagram during write and retention. (1): control oxide. (2):
nanocrystal. (3): hafnium oxide. (4): thermal oxide.
10 25A single oxide layer
10 10A oxide/62A HfO2 layer
2 D=50A, T2=50A
0 2 4 6 8 10
Figure 2.10: The bi- layer tunnel layer offers faster programming than the single tunnel
layer when the gate voltage exceeds 4.2V.
In conclusion, the low injection barrier, reduction of charging energy and deep trap
energy level obtained from high-K materials can improve nanocrystal memory
2.3.3 Semiconductor nanocrystal memory as DRAM
The analysis above shows that the semiconductor nanocrystal memory device is
promising for non-volatile memory application due to the advantages of fast
programming speed at low voltage and good retention characteristic with thin tunnel
oxide. It would be desirable if the nanocrystal memory could replace DRAM since the
processing flow for nanocrystal memory device is much simpler and nanocrystal memory
is more scalable. Nanocrystal memory with thin tunnel oxide (below 15 Å) is considered
here. The write/erase characteristic for 5nm and 3nm nanocrystal memories with 15 Å
tunnel oxide are shown in Fig. 2.11a. The retention times are shown in Fig. 2.11c.
10 T1=15A, T 2=50A
Programming time(sec) 10 D=30A
-10 -8 -6 -4 -2 0 2 4 6 8 10
Gate Voltage (V)
Figure 2.11a: Write/Erase characteristic for 15 Å tunnel oxide thickness. 10ns write
speed can’t be achieved at low programming voltage (<3V) even with larger
10 D=3nm, T2=30A
-10 D=5nm, T2=50A
10 D=5nm, T2=30A
-6 -5 -4 -3 -2 -1 0 1 2 3 4 5 6
Gate voltage (V)
Figure 2.11b: Write/Erase characteristic for 10 Å tunnel oxide thickness. 10ns write speed
can achieved at low programming voltage. Scaling the control oxide can help the write speed
at 85 C
9 10 11 12 13 14 15 16
Tunnel oxide thickness (A)
Figure 2.11c: The retention time characteristics for thin tunnel oxide thickness. 300
seconds retention time can be maintained at 10 Å, which is still better than that of
DRAM. Semiconductor nanocrystal memory could work as DRAM
Fig. 2.11a shows that it is difficult to obtain 10 ns write time at low voltage (3V),
regardless of nanocrystal diameter. Larger programming voltages (e.g. 10 V) can be used
to improve write/erase speed, of course. Fig. 2.11b shows that 10 ns write/erase times can
be achieved with 10Å tunnel oxide, for both 3nm and 5nm nanocrystal. For a 5nm
nanocrystal, scaling the top control oxide from 50 Å to 30 Å can result in sub- nanosecond
write speed at 3V. However this scaling is not recommended since it results in a small
threshold voltage (VT ) window. The refresh time at 85o C is still better than that of DRAM.
For example, the retention time of a 5nm nanocrystal memory is about 300 seconds with
10 Å tunnel oxide thickness.
Based on the above analysis, the nanocrystal memory device would work very well
as a flash-EEPROM memory device and DRAM. The semiconductor nanocrystal memory
performance will also depend on the shape of the nanocrystals as well as their crystalline
orientation, since these influence both the quantum confinement/Coulomb-charging
energy and the transmission efficiency. These variations in nanocrystal characteristics are
not considered here.
Unfortunately, semiconductor nanocrystal memory may not be the ultimate
solution to flash memory scaling, although it is a novel memory structure that still
attracts a lot of attention now. It is hard to control the uniformity of the
nanocrystals’ size and their physical locations in the channel. It is not a surprise
that nanocrystal memories exhibit large device-to-device variation .
A model based on Coulomb blockade and quantum confinement theory has been
developed to predict the write/erase speed of nanocrystal memory devices and to serve as
a guide for their design. A trap model is proposed to describe the retention. Germanium
nanocrystal memory devices can provide at least 106 times larger retention-time to write-
time ratio than conventional floating- gate devices. The optimum nanocrystal size is
around 5nm. High-K, low barrier tunnel materials such as nitride can enhance the
performance further. Nanocrystal memory could also work as a DRAM, although the
retention time enhancement may not be significant enough.
 Y. King, “Thin Dielectric Technology and Memory Devices”, Ph.D thesis, UC,
 S. Tiwari, F. Rana, K. Chan, H. Hanafi, W. Chan and D. Buchanan, “Volatile and
Non-Volatile Memories in Silicon with Nano-Crystal Storage,” IEDM Technical
Digest, p. 521, 1995.
 I. Kim, S. Han, K. Han, J. Lee and H. Shin, “Room Temperature Single Electron
Effects in a Si Nano-Crystal Memory,” IEEE Electron Device Letters, Vol. 20, No. 12,
 Y. King, T.-J. King and C. Hu, “MOS Memory Using Germanium Nanocrystals
Formed by Thermal Oxidation of Si1 -x Gex ”, IEDM Technical Digest, p.115, 1998.
 H. Grabert and Michel H. Devoret, “Single charge tunneling: Coulomb blockade
phenomena in nanostructures,” New York: Plenum Press, 1992.
 “Quantum Mechanical CV Simulator”, available at http://www-
 J.D.Jackson, “Classcial Electrodynamics”, published by John Wiley & Sons, 1999.
 T. Takagahara and K.Takeda, “Theory of the quantum confinement effect on excitons
in quantum dots of indirect- gap materials,” Phys. Rev. B, Vol. 46, p. 15578, 1992.
 Y. Niquet, G. Allan, C. Delerue and M. Lannoo, “Quantum confinement in germanium
nanocrystals”, Applied Physics Letters, Vol. 77, p.1182, 2000.
 K. L. Teo, S. H. Kwok, P.Y.Yu and S.Guha, “
Quantum Confinement of the Two-
Dimensional E1 Excitons in Ge Nanocrystals “, unpublished.
 S. Y. Ren, “Quantum Confinement in Semiconductor Ge Quantum Dots”, Solid
State Communications, Vol.102, p.479, 1997.
 B. De Salvo et al, “Experimental and Theoretical Investigation of Nonvolatile
Memory Data-Retention, IEEE Transactions on Electron Devices, Vol.46, No.7, 1999.
 Y. Shi, Private communication, Nanjing University.
 E.H .Nicollian, “MOS Physics and Technology”, published by John Wiley & Sons,
 M. She, T.-J. King, C. Hu et al, “JVD Silicon Nitride as Tunnel Dielectric in P-
channel Flash Memory”, IEEE Electron Device Letters, pp.91 -93, Vol. 23, Issue 2,
 D.W.Kim, F.E.Prins, T.Kim, D.L.Kwong and S.Banerjee, “Charge Retention
Characteristics of SiGe Quantum Dot Flash Memories”, 60th Device Research
 K.Likharev, “Layered Tunnel Barriers for Nonvolatile Memory Devices”, Applied
Physics Letters, Vol.73, No.15, p.2137, 1998.
 Govoreanu, B.; Blomme, P.; Rosmeulen, M.; Van Houdt, J.; De Meyer, K.
“VARIOT: a novel multilayer tunnel barrier concept for low-voltage nonvolatile
memory devices”, IEEE Electron Device Letters, pp.99-101, Vol.24, Issue 2, 2003.
Low barrier tunnel dielectrics for flash
Thermal silicon dioxide has been used as the tunnel dielectric since the invention of
flash memory. Low voltage operation requires the tunnel oxide thickness to be scaled.
However, it is difficult to reduce the tunnel oxide thickness below 7nm, if 10 years
retention time is desired. In this chapter, low tunnel barrier dielectric such as silicon
nitride is investigated as an alternative tunnel dielectric to make flash memory more
3.2 JVD nitride as a tunnel dielectric in floating gate flash
In this section, Jet Vapor deposited nitride  is used as a tunnel dielectric in the
flash memory. The hot electron injection barriers of the tunnel oxide and the JVD tunnel
nitride are 3.15eV and 2.12eV, respectively. Hence electron injection is much more
efficient, and fast programming can be achieved at low operation voltage, if the tunnel
dielectric is JVD nitride.
In a conventional flash memory device programmed by hot-electron injection, the
electrons must have energy close to or higher than that of the oxide barrier (3.15eV) to be
injected into the floating gate. A very small percentage of electrons in the channel have
such high energy, as shown in Fig. 3.1 , so the current injected into the floating gate is
very small, resulting in slow programming. High voltages are required to produce these
hot electrons, so it is difficult to scale the program/erase voltages with each technology
node. A low-barrier tunnel dielectric is therefore necessary to improve programming
efficiency and speed with the possibility of reducing the operating voltages.
electron distribution (a.u)
0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5
electron energy (eV)
Figure 3.1: The electron energy distribution in the channel near the drain side.
L=0.5um, Tox =10nm, VGS=1.5V and VDS=3V . The majority of the electrons have
energy lower than 3.15eV.
Recently, JVD (jet vapor deposited) nitride has been demonstrated to be a promising
high-quality gate dielectric for future CMOS technologies  since it offers smaller gate
leakage current and reduced stress-induced leakage current compared to SiO 2 gate
dielectric. Due to its low barrier for electrons (2.12eV), JVD nitride can be used as the
tunnel dielectric in a flash memory device in order to enhance hot-electron injection and
thereby improve the programming speed. Since the tunneling barrier for holes is only
1.9eV, hot hole injection can be used for erasing with appropriate operating voltages. In
this work, the performance characteristics of the first p-channel flash memory devices
with JVD nitride tunnel dielectric are presented. P-channel flash memory devices offer
several advantages over their n-channel counterparts: lower power, higher speed and
better reliability . As compared with co- fabricated control devices with thermal silicon
dioxide tunnel die lectric of the same equivalent oxide thickness, the JVD nitride devices
show markedly better performance.
3.2.2 Hot carrier injection efficiency
Although the hot carrier injection phenomenon in CMOS devices has been studied
for a long time, it is still difficult to model the injection current accurately. In this section,
the lucky electron model of channel hot electron injection developed by Hu  and the
hot electron injection current model developed by Sonada  are employed to
qualitatively study the programming efficiency in the floating gate flash memory.
Figure 3.2: Cross-section of a
Floating gate floating gate flash memory
device. The hot electron injection
Tunnel oxide B process is illustrated with arrows.
For an electron to be injected into the floating gate, it needs to acquire enough
kinetic energy (φ 0 =3.15eV) to surmount the tunnel oxide barrier. The channel electron
gains kinetic energy from the lateral channel electrical field and becomes “hot” when it
accelerates from the source side to the drain side (location A) under positive drain bias.
The lateral electric field reaches its maximum near the drain region. This is why the hot
electron injection always happens near the drain side. Assuming the lateral electrical field
is Em at the drain, the electrons must travel a distance of φ 0 /Em to acquire kinetic energy
of φ 0. However, during the acceleration, the electrons will encounter optical phonon
scattering and lose their kinetic energy. Only some lucky electrons can avoid the
scattering and acquire enough kinetic energy. If the mean free path associated with the
phonon scattering is λ , the probability for a lucky electron to acquire kinetic energy of
φ 0 or more is e ( −φ 0 / E m λ ) .
For an electron to be injected into the floating gate, its momentum must be redirected
towards the substrate/ tunnel oxide interface and the electron will move from location A
to location B (location B is at the interface). After that the electron will be swept into the
floating gate if the electric field across the tunnel oxide favors its injection. The
probability of an electron acquiring the kinetic energy φ 0 or more and retaining the
appropriate momentum after re-direction  is
E m λ ( −φ0 / E m λ )
p0 = e (3.1)
After integrating the injection probability and the current along the channel, the hot
electron injection current is expressed as:
λEm 2 ( −φ b / E m λ )
I inj = Ad I ds ( ) e (3.2)
Here I ds is the channel current and Ad is a constant . If the injection barrier φ b is
reduced, the injection current will increase exponentially according to Equation (3.2).
Since JVD nitride offers a small injection barrier, flash memory with a JVD tunnel layer
can be programmed faster than the memory with an oxide tunnel layer.
3.2.3 Retention and erase
Control Floating gate EC
Figure 3.3: The energy band diagram during retention. Only the conduction band edge
is shown here. The electrons in the floating gate can leak back to the channel due to
the internal electric field induced by the charges in the floating gate.
During retention, electrons could tunnel back to the channel, constituting a large
leakage current. The magnitude of the leakage current depends on both the thickness and
the electron barrier height of the tunnel dielectric. The tunneling probability is expressed
d φ ( x) * me
T = exp( −2 ∫ dx ) (3.3)
Here, d is the dielectric thickness. me is the electron mass inside the tunnel dielectric and
it is 0.5m0 for both nitride and oxide. Since the electrons will raise the floating gate
potential, there is small voltage drop V across the tunnel dielectric. V is the floating
gate potential relative to the channel during retention mode. The tunneling probability is
calculated in terms of V0 , as shown in Fig. 3.4(a).
During retention, the control gate, source/drain and body are grounded. V0 will be
about 2V if the threshold voltage shift between the programmed state and the erased state
is 3V, assuming the coupling ratio of the memory device is 0.65 . Since the voltage
drop is smaller than the 3.15eV electron injection barrier, the electrons leak away via
“direct tunneling” during retention. The tunneling probability depends very weakly on the
electron barrier height but strongly on the tunnel dielectric thickness. As shown in Fig.
3.4(a), the leakage current through an 8nm tunnel nitride is about four orders of
magnitude lower than that through a 5nm tunnel oxide at a V0 of 2V, and as a result the
retention time is greatly enhanced. The technique of biasing the control gate during
retention can be applied to enhance the retention time for floating gate flash memory. If
the control gate bias is set at 3V during retention, V0 will be 0V. Then the leakage current
through an 8nm tunnel nitride is more than ten orders of magnitude lower than that
through a 5nm tunnel oxide.
Tunneling probability T
-18 φ (0)
10 FG Tunnel
10 5nm Oxide dielectric
10 8nm Nitride
10 12nm Nitride
0 2 4 6 8
Figure 3.4: (a) The tunneling probability comparison. (b) The energy band
diagram during erasing. 51